text: Pouring metal defects include misruns, cold shuts, and inclusions. A misrun occurs when the liquid metal does not completely fill the mould cavity, leaving an unfilled portion. Cold shuts occur when two fronts of liquid metal do not fuse properly in the mould cavity, leaving a weak spot. Both are caused by either a lack of fluidity in the molten metal or cross-sections that are too narrow. The fluidity can be increased by changing the chemical composition of the metal or by increasing the pouring temperature. Another possible cause is back pressure from improperly vented mould cavities.
  Misruns and cold shuts are closely related and both involve the material freezing before it completely fills the mould cavity. These types of defects are serious because the area surrounding the defect is significantly weaker than intended. The castability and viscosity of the material can be important factors with these problems. Fluidity affects the minimum section thickness that can be cast, the maximum length of thin sections, fineness of feasibly cast details, and the accuracy of filling mould extremities. There are various ways of measuring the fluidity of a material, although it usually involves using a standard mould shape and measuring the distance the material flows. Fluidity is affected by the composition of the material, freezing temperature or range, surface tension of oxide films, and, most importantly, the pouring temperature. The higher the pouring temperature, the greater the fluidity; however, excessive temperatures can be detrimental, leading to a reaction between the material and the mould; in casting processes that use a porous mould material the material may even penetrate the mould material.
  The point at which the material cannot flow is called the coherency point. The point is difficult to predict in mould design because it is dependent on the solid fraction, the structure of the solidified particles, and the local shear strain rate of the fluid. Usually this value ranges from 0.4 to 0.8.
  An inclusion is a metal contamination of dross, if solid, or slag, if liquid. These usually are impurities in the pour metal (generally oxides, less frequently nitrides, carbides, or sulfides), material that is eroded from furnace or ladle linings, or contaminates from the mould. In the specific case of aluminium alloys, it is important to control the concentration of inclusions by measuring them in the liquid aluminium and taking actions to keep them to the required level.
  There are a number of ways to reduce the concentration of inclusions. In order to reduce oxide formation the metal can be melted with a flux, in a vacuum, or in an inert atmosphere. Other ingredients can be added to the mixture to cause the dross to float to the top where it can be skimmed off before the metal is poured into the mould. If this is not practical, then a special ladle that pours the metal from the bottom can be used. Another option is to install ceramic filters into the gating system. Otherwise swirl gates can be formed which swirl the liquid metal as it is poured in, forcing the lighter inclusions to the center and keeping them out of the casting. If some of the dross or slag is folded into the molten metal then it becomes an entrainment defect.